Download presentation

Presentation is loading. Please wait.

Published byHugo Lynch Modified about 1 year ago

1
Single Crystal Slip Adapted from Fig. 7.8, Callister 7e. Adapted from Fig. 7.9, Callister 7e.

2
Calculation of Theoretical Shear Stress for a Perfect Lattice G. Dieter, Mechanical Metallurgy, 3rd Edition, McGraw-Hill, 1986.

3
Dislocation Concept Concept of dislocation was first introduced to explain the discrepancy between observed and theoretical shear strengths For the dislocation concept to be valid: 1.The motion of a dislocation through a lattice must require less stress than the theoretical shear stress 2.The movement of dislocations must produce steps or slip bands at free surfaces

4
Cottrell Energy Argument Plastic deformation is transition from unslipped to slipped state The process is opposed by an energy barrier To minimize energy the slipped material will grow by advance of an interfacial region (dislocation) To minimize energy of transition – interface thickness, w, small Distance w is width of dislocation –Smaller w – lower interfacial energy –Larger w – lower elastic energy of the crystal – atomic spacing in the slip direction is closer to atomic spacing Equilibrium width is a balance of these two components G. Dieter, Mechanical Metallurgy, 3rd Edition, McGraw-Hill, 1986.

5
Peierls-Nabarro Force Dislocation width determines the force required to move a dislocation through a crystal lattice Peierls stress is the shear stress required to move a dislocation through a crystal lattice Note: wide dislocations require lower stress to move –Makes sense: Wide – the highly distorted region at core is not localized on any particular atom In ductile metals the dislocation width is on the order of 10 atomic spacings a is distance between slip planes b is the distance between atoms in the slip direction In ceramics with directional covalent bonds – high interfacial energy, dislocations are narrow – relatively immobile Combined with restrictions on slip systems imposed by electrostatic forces – low degree of plasticity

6
Dislocation Motion Covalent Ceramics (Si, diamond): Motion hard. -directional (angular) bonding Ionic Ceramics (NaCl): Motion hard. -need to avoid ++ and - - neighbors. ++++ +++ ++++ --- ---- --- Metals: Disl. motion easier. -non-directional bonding -close-packed directions for slip. electron cloudion cores + + + + +++++++ + +++++ +++++ + +

7
Dislocation Motion Dislocations & plastic deformation Cubic & hexagonal metals - plastic deformation by plastic shear or slip where one plane of atoms slides over adjacent plane by defect motion (dislocations). If dislocations don't move, deformation doesn't occur! Adapted from Fig. 7.1, Callister 7e.

8
Dislocation Motion Dislocation moves along slip plane in slip direction perpendicular to dislocation line Slip direction same direction as Burgers vector Edge dislocation Screw dislocation Adapted from Fig. 7.2, Callister 7e.

9
–Slip plane - plane allowing easiest slippage: Minimize atomic distortion (energy) associated with dislocation motion Wide interplanar spacings - highest planar atomic densities (Close Packed) –Slip direction - direction of movement Highest linear atomic densities on slip plane Definition of a Slip System

10
Independent Slip Systems –The number of independent slip systems is the total possible number of combinations of slip planes and directions Example: FCC –Slip occurs on {111} planes (close-packed) in directions (close- packed) –4 Unique {111} planes –On each plane 3 independent ‹110› –Total of 12 slip systems in FCC

11
Slip Systems Some slip systems in BCC are only activated at high temperatures BCC and FCC have many possible slip systems – ductile materials HCP: Less possible slip systems – brittle material

12
Stress and Dislocation Motion Crystals slip due to a resolved shear stress, R. Applied tension can produce such a stress. slip plane normal, n s Resolved shear stress: RR =F s /A/A s slip direction ASAS RR RR FSFS slip direction Relation between and RR RR = FSFS /AS/AS Fcos A/cos F FSFS nSnS ASAS A Applied tensile stress: = F/A slip direction F A F

13
Condition for dislocation motion: Crystal orientation can make it easy or hard to move dislocation 10 -4 GPa to 10 -2 GPa typically Critical Resolved Shear Stress maximum at = = 45º RR = 0 =90° RR = /2 =45° RR = 0 =90° Schmid’s Law Schmid Factor

14
Ex: Deformation of single crystal So the applied stress of 6500 psi will not cause the crystal to yield. =35° =60° crss = 3000 psi a) Will the single crystal yield? b) If not, what stress is needed? = 6500 psi Adapted from Fig. 7.7, Callister 7e.

15
Ex: Deformation of single crystal What stress is necessary (i.e., what is the yield stress, y )? So for deformation to occur the applied stress must be greater than or equal to the yield stress

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google